Optimization of cold forging process technology by means of simulation Hendrik Muntinga Hendrik Muntinga Ingenieurbro, Rosenthal, Herscheid Nikolai Biba, Sergei Stebunov QuantorForm Ltd, Moscow, Russia Abstract: The paper presents an approach to increasing of cold and warm forging process quality and economical efficiency by means of computer simulation. The main ways for achieving of stable product quality, long tool life and high accuracy are analysed. The technology improvement is reached by modification of perform and die design that eliminates flow induced defects, reduces stress concentration in critical areas through optimising of fillets and/or introducing splits in combination with shrink rings and hard inserts. Finite element simulation allows finding optimal value of interference that provides compressive stress state in hard but fragile inserts under actual forging load. Simulation also generates profiled shape of the die that compensates elastic deformation of tooling set and provides precise geometrical accuracy of a forged part. Ductile fracture of the forged part can be predicted and minimised by means of simulation. Presented model is realised in commercial metal forming simulation program QForm. 1. Introduction
Besides of great advantages, cold forging technology has drawbacks that make its implementation sometimes difficult. They are:
Potentially higher contact stress that may cause tool fail or excessive tool deflection Probable fracture due to deformation limit of cold material
Nevertheless the practice shows that these drawbacks can be minimised by means of
Optimal design of preforming operations to avoid flow induced defects, reduce contact stress and fracture probability
Optimisation of die assembly to provide longer tool life and to keep die deflection within tolerance
Numerical simulation is the most effective way to reduce the cost and development time
required for such optimisation. Meanwhile specifics of cold forging apply special requirements to the simulation software. Particularly they are:
Especially effective automatic adaptive remeshing is necessary for simulation of the
material flow in the dies with small fillet radii that are typical for cold forging Advanced capabilities for simulation of complex pre-stressed tool sets are required as a
routine option including tool life prediction due to cycle fatigue and die wear Reliable damage prediction facilities are necessary for optimal design of preform shapes
to reduce fracture probability Forging simulation program QForm developed by QuantorForm Ltd.  completely fulfils the above requirements. The program is based on the most modern and sophisticated programming technique and advanced FEM algorithms. QForm is the next generation forging simulation software and has the following main features:
QForm is object-based and naturally integrated with Windows environment. Graphical interface makes it clear and easy even for PC users of begin level.
The user operates the program for simulation of 2D and 3D problems through the same interface.
Completely integrated architecture of QForm provides synchronous work of all parts of the program (all-in-one design). Pre-processing is performed in parallel with source data preparation that makes users work vivid and understandable. The user is guided by so-called Data Preparation Wizard that eliminates possible mistakes or missed data.
Meshing and re-meshing is absolutely automatic and the program never requires users interference during simulation. There is no access to specific simulation control parameters in QForm at all. It makes accuracy of simulation independent of users qualification.
Post-processing is performed concurrently with the progress of simulation that allows immediately to interpret the results.
The user works not just with simulation of a single forming operation (blow) but with complete technological chain that includes the sequence of blows separated by intermediate cooling/heating or clipping/piercing operations. Simulation of such technological chain is performed automatically without users interventions that makes what if analysis very fast and effective.
Reliable and accurate import of source geometrical data from CAD systems through STEP and IGES formats as well as direct interface.
Facilities to pierce the holes and trim the flash between forming operations. Manual and automatic positioning of the workpiece on the dies. Simulation of workpiece motion as a rigid body subject to gravity, friction and inertia
to find out its stable position before forming simulation (gravitational positioning).
The software is easy to learn and very reliable in everyday use. The user friendliness of QForm is boosted by effective remote support via Internet that works perfectly regardless of distance between the user and the supplier and ensures minimal time losses. 2. Material flow optimisation in cold and warm forging 2.1. Avoiding laps In certain conditions of deformation the material can buckle causing collapse of free surface resulting in laps and folds. Laps are the defects that appear when free surface of material folds over itself. From practical point of view the laps are very annoying kind of defects because they tend to appear each time when we want to intensify deformation for cost reduction, for example, when we try to skip preforming operation. The lap can occur in rib-web forging at a variety of locations where the rib may buckle. Sometimes laps can appear when we try to upset a billet with diameter to height ratio within admissible limit but due to small deviations from ideal shape or non-parallel cuts the billet may buckle. The fully automatic finite element mesh generation implemented in QForm ensures simulation of surface-to-surface contact that happens in a lap area. It is very important for reliable prediction of this defect. The program automatically increases mesh density in critical area when the surface starts to collapse. This feature is illustrated by practical example of warm forging of the cam of oval shape with two round off-centre cavities of different depth. This is 3D problem. When using cylindrical billet the material first fills the shorter arm of the cam and then flows in circumferential direction towards its long arm and the laps occur on its upper and lower surfaces (Fig 1 b). The pin on the lower die is higher than on the upper die and lower lap is more developed then upper one. The program automatically detects the zones where the lap potentially may occur and automatically increases the mesh density there (Fig 2.b). Thus the program is able to detect the finest peculiarities of the material flow and is very sensitive.
a. b. Fig.1. Cam forging using cylindrical billet (a). The laps are shown in the boxes (b).
a. b. Fig. 2. Cam forging. Mesh density increases in the zones where the laps occur (in the boxes). To avoid the laps the billet should be upset and then placed into the die. Meanwhile the height of upsetting is the question because the billet must fit into the die as accurate as possible. It is difficult to guess the optimal height just using volume constancy rule because of barrelling the billet may not fit the dies as shown on Fig. 3.
a. b. Fig. 3. The upset billet that does not fit the dies: front view (a) and top view (b).
Using QForm it is easy to select the height of upsetting that allows the billet to fall into the die. To be the most close to reality the program also can simulate gravitational motion of the billet that allows to find its stable position on the lower die (Fig.4).
Fig. 4. Optimal shape of the billet after upsetting that provides its stable position in the lower die: front view (a) and top view (b). The simulation has shown that using upset billet that exactly fits the die the material flows without laps providing the product of sound quality (see Fig. 5b comparing to Fig 1b).
a. b. Fig. 5. Forging of the cam using upset billet: initial position of the billet (a) and its final shape (b). 2.2. Detecting and fixing flow-through defects Flow-through defect occurs when the material is forced to flow past a recess after it was filled or regions that have stopped to deform because of chilling. As written in  Similar to laps in appearance, flow-through defects may be shallow but indicative of an undesirable grain flow patterns or shear band that extends much father into the forging. It is important that in flow-through defect there is no collapse of free surface. Meanwhile this kind of defect can be reliably detected by means of simulation. Let us investigate a forging defect that appears in aluminium part produced in one blow. This is round part and can be simulated in 2D. The picture on Fig. 6,a shows its cross cut. There is a circular defect around the central area that looks like a crack or, maybe, a lap. The shape of the defect is better seen on magnified right picture (Fig 6,b). Thus just looking at polished cross cut it is difficult to say what particular kind of the defect we have, how to classify it (crack, lap or flow-though defect) and how to fix it.
On the picture of macrostructure (Fig. 6a) we see the zone of extremely intensive shearing deformation that begins from the defect. It means that the defect was caused by intensive shearing deformation. The small crack (Fig. 6b) is just visible part of the defect while it goes deep into the billet body.
a. b. Fig. 6. Cross cut of aluminum part after surface etching. General view (a) and the area in the box that is magnified to show the de